New Layered Materials: Syntheses, Structures, and Optical Properties of K2TiCu2S4, Rb2TiCu2S4, Rb2TiAg2S4, Cs2TiAg2S4, and Cs2TiCu2Se4
Fu Qiang Huang; James A. Ibers; Inorganic Chemistry 40 (2001) 2602–2607; doi:10.1021/ic001346d

data_4319681
_publ_section_title
;
 New Layered Materials: Syntheses, Structures, and Optical Properties of
 K2TiCu2S4, Rb2TiCu2S4, Rb2TiAg2S4, Cs2TiAg2S4, and Cs2TiCu2Se4
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2602
_journal_page_last               2607
_journal_paper_doi               10.1021/ic001346d
_journal_volume                  40
_journal_year                    2001
_chemical_formula_sum            'Cu2 Rb2 S4 Ti'
_chemical_formula_weight         474.16
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           132
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4c 2c'
_symmetry_space_group_name_H-M   'P 42/m c m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   5.6046(4)
_cell_length_b                   5.6046(4)
_cell_length_c                   13.1541(13)
_cell_measurement_temperature    153(2)
_cell_volume                     413.19(6)
_computing_cell_refinement       'SMART version 5.054 (Bruker, 2000)'
_computing_data_collection       'SMART version 5.054 (Bruker, 2000)'
_computing_data_reduction        'SAINT-Plus version 6.02A (Bruker, 2000)'
_computing_molecular_graphics    'SHELXTL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      153(2)
_diffrn_measured_fraction_theta_full 0.972
_diffrn_measured_fraction_theta_max 0.972
_diffrn_measurement_device_type  'Bruker Smart 1000 CDD'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'standard-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0253
_diffrn_reflns_av_sigmaI/netI    0.0105
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            3074
_diffrn_reflns_theta_full        28.47
_diffrn_reflns_theta_max         28.47
_diffrn_reflns_theta_min         3.10
_diffrn_standards_decay_%        <2
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    18.659
_exptl_absorpt_correction_T_max  0.159
_exptl_absorpt_correction_T_min  0.064
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    3.811
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             436
_exptl_crystal_size_max          0.184
_exptl_crystal_size_mid          0.146
_exptl_crystal_size_min          0.144
_refine_diff_density_max         1.335
_refine_diff_density_min         -0.863
_refine_diff_density_rms         0.167
_refine_ls_extinction_coef       0.0055(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.512
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         309
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.512
_refine_ls_R_factor_all          0.0227
_refine_ls_R_factor_gt           0.0220
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc 
 [1.00000+0.00000exp(0.00(sin\q/\l)^2^)]/ 
   [\s^2^(Fo^2^)+0.0000+0.0000*P+(0.0400P)^2^+0.0000sin\q/\l] 
 where P = 1.00000Fo^2^ + 0.00000Fc^2^ 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0708
_refine_ls_wR_factor_ref         0.0711
_reflns_number_gt                299
_reflns_number_total             309
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic001346d_1.cif
_cod_data_source_block           rbticus
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4319681